Outline Motivation – BSO is an alternative option; – Heavier and longer wavelength(~480nm). – Checked Light Output of small samples quickly. Set up ADC distribution – PureCsI – BSO Compared with PureCsI Summary and plans
Set up PMT : H3167(19mmφ) Borosilicate glass window Bialkali photocathode HV 1650V Scintillator PMT Radiation source 137Cs(662keV) AMPDivAMPATT DiscriG.G. Charge-sensitive ADC(LeCroy2249W) Width 500ns Veto 1ms Optical grease Threshold 20mV 30mV To match ADC range
Samples PureCsI 1φ×2cm BSO 1*1*2cm 3 BSO both ends mirror polish, 4 side surfaces are frosted. Wrapped by white Gore-TeX film.
ADC distributionof PureCsI Size : 1φ×2cm. (λ=330nm) Around photoelectric peak is magnified as right figure, together with fitted line by Gaussian. Photoelectric peak Compton scattering
ADC distribution of BSO Size : 1cm×1cm×2cm. (Purity 99.9999%, λ=480nm) ATT 6dB : To adjust ADC range. Right figure is magnification around photoelectric peak. Compton scattering Photoelectric peak
To compare with PureCsI L.O. of BSO is two times as PureCsI. Sample L.O. (PureCsI equal 1 ) BSO SA, SB and No.1 are different samples; all purity 99.9999%.. As for Pr:LuAG, see 2008 Dec. meeting slides BSO exhibits double effective L.O. because of longer wavelength!
Comments on sample dimension and surface finishing. Light collections for PureCsI(cylindrical)=BSO(1X1X2cm 3 ) assumed. In order to make sure, PureCsI (1X1X2cm 3 ) ordered, delivered in 3 weeks. Then answer becomes clearer.
Actually we experienced; L.O. of 2x2x2cm 3 BSO(all 6 surfaces mirror polished) exhibits ~ half of 1x1x2cm 3 (only both end surfaces are mirror polished) sample. – Though they are taken from the exactly same block. Thought to because of photons total reflection at its polished surfaces ~45 deg. Significant amount of photons are absorbed during travel inside crystal… x Common phenomena in crystal with n>sqrt(2).
Summary and plans Effective L.O. of BSO is 2 times as high as PureCsI because of longer wavelength. 1*1*2cm 3 PureCsI (Both ends mirror polish, 4 side surfaces are frosted) will be gotten soon. – To remove possible light collection difference. Radiation hardness test of BSO(and Pr:LuAG) small samples.